1 Steel Making Prof. Deepak Mazumdar Prof. S. C. Koria Department of Materials Science and Engineering Indian Institute of Technology, Kanpur Module No. # 01 Lecture No. # 19 Modern Steelmaking II, Electric Arc Furnace In the last lecture, I have said about stainless steel making in electric arc furnace. I have also said, the different types of stainless steel which are to be manufactured for different applications. I have also said, because of the limited availability of high quality stainless steel scrap, it has become important to use high carbon ferrochrome, required to decarburize iron chromium melt, because most of the stainless steel applications for most of the applications, they require carbon in a very low range. (Refer Slide Time: 01:23) So, therefore, use of high carbon ferrochrome required the decarburization of iron, chromium, carbon containing melt. I have also said, that decarburization in presence of chromium, can only occur at very high temperature. If we blow oxygen, until that high temperature reaches, chromium oxidizes in preference to carbon. I have also said at that
2 time, that we have to find out a temperature at which carbon oxidation begins in preference to chromium oxidation. In that connection, I had given you two equations and those equations I have again written for you, that is the equation a, it tells the distribution of chromium and carbon as a function of temperature and partial pressure of carbon monoxide for iron, chromium and carbon melt. If the melt has nickel also, nickel increases the activity coefficient of carbon. So, therefore, an another equation was proposed for decarburization of iron, chromium, carbon and nickel melt and this equation is shown in b. Now, let us today illustrate the effect of temperature and partial pressure of carbon monoxide for two different melts. What I am doing, I will be taking the different temperature; I will be also taking different partial pressure of carbon monoxide to illustrate to the effect of temperature and partial pressure of carbon monoxide; then I will take an example for iron, chromium and carbon melt and I will also take an example of iron, chromium, carbon and a constant nickel, for example, 10 percent nickel. (Refer Slide Time: 03:14) Now, as regards the calculation procedure, I have presented over here. I take temperature. Then, I have taken iron, chromium, carbon melt and I will calculate the ratio of percentage chromium upon percentage carbon in melt. Next, I will calculate for the same temperature, the ratio of weight percent chromium upon weight percent carbon in melt, for iron, chromium, carbon and nickel. I am illustrating for a constant percent
3 nickel, for example, 10. You can calculate, for example, for 12 or 14 or whatever, if the need arises. So, what I am doing, I am using the equations a and b for that calculation purposes. So, suppose, I take temperature 1873 Kelvin which is 1600 degree Celsius, I substitute that value and I put p C O is equal to 1 atmosphere, then I will be calculating this ratio as 25 and here this ratio is 36. If I take now, a temperature 1973 Kelvin, which is equal to 1700 degree Celsius, then the ratio is 58 for iron, chromium, carbon melt and the ratio is 82 for iron, chromium, carbon and nickel melt. If I take a temperature now of 2073 Kelvin, which is 1800 degree Celsius, then the ratio becomes 128 and here 172. If I take the temperature 2173 Kelvin, which is equal to 1850 degree Celsius, the ratio becomes 240 and here it becomes 339. Now, mind you, these calculations are performed by taking partial pressure of C O that is equal to 1 atmosphere. What this calculation says? Increase in temperature increases the ratio of chromium to carbon in the melt, that I am going to write, increase in temperature, increase in temperature, increases percent chromium in metal upon percent carbon in metal. So, for example, if I take 1600 degree Celsius as my temperature, then the ratio is only 25. If I take now 1850 degree Celsius, the ratio is 240, which increases, when nickel is there to 339. So, another is that, for a given temperature, the ratio percent chromium upon percent carbon in melt, it increases with nickel content. Reason is obvious, because nickel increases the activity coefficient of carbon. So, now, let me illustrate, what is the effect of when we decrease the partial pressure of carbon monoxide.
4 (Refer Slide Time: 06:53) Now, the same thing, I take now partial pressure of carbon monoxide say 0.25 atmosphere. Again I take here, temperature and the ratio of percentage chromium upon percentage carbon for iron, chromium and carbon melt and percentage chromium upon percentage carbon in the melt for iron, chromium, carbon and nickel. Temperatures, again I take 1873, 1973, 2073 and The ratio here is 89, 209, 460 and 863. Here 129, 295, 619 and So, you see, decrease in partial pressure of carbon monoxide from 1 atmosphere to 0.25 atmosphere, it increases the ratio of percentage chromium upon percentage carbon in the melt for all temperatures. Now, if I take for example, further I reduce the pressure. So, I do p C O is equal to 0.1 atmosphere. So, these are for p C O is equal to 0.1 atmosphere and I again calculate for all the four temperatures, then the ratio becomes 207, 488, 1077 and Here it becomes 301, 690, 1447 and So, what this calculation indicates? This calculation indicates, if we reduce the partial pressure of carbon monoxide, then the ratio of percent chromium upon percentage carbon, it increases drastically.
5 (Refer Slide Time: 09:27) (Refer Slide Time: 09:35) If I take p C O is equal to 1 atmosphere for example, if I take p C O is equal to 1 atmosphere at 2073 Kelvin, the ratio is 128. The same ratio becomes 460, when p C O is 0.25 atmosphere and the same ratio becomes 1077, when p C O is equal to 1 atmosphere. That means now, by decreasing the partial pressure of carbon monoxide, I can increase this ratio; that means, I can allow now carbon reaction to proceed at much lower temperature. So, that is what the importance of temperature and partial pressure of carbon monoxide.
6 So, what we gather or what the scientific calculation suggest us, that, if you want to carry out decarburization of iron, chromium, carbon, nickel melt at partial pressure of carbon monoxide is equal to 1 atmosphere, then the decarburization is only possible at a very high temperature. Now, this temperature can be reduced, when you decrease the partial pressure of carbon monoxide. The extent of reduction of this temperature will depend upon, the extent of reduction of the partial pressure of carbon monoxide. If you can lower down further the partial pressure of carbon monoxide, for example, you make stainless steel under vacuum and pressure is very low, then, the decarburization can be carried out still at lower temperature. So, this is an important conclusion of this particular calculation, as far as the effect of temperature and partial pressure of carbon monoxide is concerned. (Refer Slide Time: 11:30) Now, another important thing, in this particular case, also, how to make now use of these calculations in the stainless steel making. So, let us see, first of all, melting of scrap in, melting of stainless steel scrap in E A F, in the light of knowledge that we have gathered previously. So, charge, it consists of S S scrap plus carbon steel scrap plus lime. Mind you, the melting of S S scrap in E A F is carried out at atmospheric pressure. So, p C O is that 1 atmospheric pressure. After charging, same, melt down, the charge is molten in the melt down period and at the melt down period the bath contains, for example, 10 percent chromium, all nickel which you have charged, plus carbon.
7 Now, oxygen is blown into iron, chromium, nickel, carbon melt. Unless the temperature rises, the carbon oxidization does not begin. So, lot of chromium gets oxidized. Oxidation of chromium is exothermic reactions. Temperature of the bath rises and then, carbon also begin to decrease. So, initially chromium oxidizes until bath temperature rises to 1800 degree Celsius. Above 1800 degree Celsius, carbon begins to oxidize. So, what is important here is that, higher chromium content at the end of melt down stage will require higher temperature, as already we have seen in the calculation. So, what is important, at the melt down stage that the chromium content, I should not say too low, but it should not be very high, because then you will be requiring very high temperature for carbon to oxidize. So, when this practice, when this has been attained, a decarburization has occurred, then, in the finishing stage, balance chromium is added, as low carbon ferrochrome and then, the heat is finished. It is tapped and well, cast and so on and so forth. Now, this particular technology was working for a long time, but there are certain limitations of this technology. The first limitation of this technology is use of low carbon ferrochrome. Second effect, as a result of high temperature working in electric arc furnace is at high temperature, damages the refractory lining. Third important point is this. A complete heat, a complete heat, it takes about 8 hours from charging to finishing. We require a stainless steel at a reasonable cost. These limitations or that technology using electric arc furnace, made this stainless steel cost high. What is to be done? It is a challenge to the technologist and these limitations that were imposed in electric arc furnace steelmaking paved the way to find out an alternative technology.
8 (Refer Slide Time: 16:45) The basis of alternative technology is, basis of alternative technology is, one to carry decarburization at low temperature. This is one particular challenge or one particular basis of development of a new technology, to carry decarburization at low temperature without oxidation of chromium. Second, as repeatedly I have said, low carbon ferrochrome is very expensive and hence, high carbon ferrochrome, if it can be used for production of a stainless steel containing high chromium, then it will be economical. So, the second challenge was, use of high carbon ferrochrome. What is the scientific solution? The scientific solution is that, if carbon is to be oxidized in preference to chromium at a given temperature, what we should do it? I have just told you the role of partial pressure of carbon monoxide. I have also illustrated what happens, if I reduce the partial pressure of carbon monoxide. In the earlier calculation I have shown you, that deduction of partial pressure of carbon monoxide increases the ratio of chromium to carbon in the melt and as a result I can produce a low carbon without causing oxidation of chromium. That is what the calculation we have seen. So, what is the solution? To oxidize the carbon in preference to chromium, we must aim at the reduction of partial pressure of carbon monoxide below 1 atmosphere. For example, whatever you can reduce, you will gain in deduction in the temperature, 1, 2.5, 2.25 or 0.1, as you see in the calculation, then this is possible. Simple. We can also see, for example, if I write down the reaction 2 C plus O 2 that is equal to 2 C O. 1 mole of
9 oxygen it produce 2 moles of C O. So, obviously, decrease in pressure will favor carbon oxidization in presence, for example, if I have 4 by 3 chromium plus O 2 that is equal to two third chromium oxide. I need not want to carry out the calculation. Just, I have to see both these equations, and if I see both these equation, in the equation one there is a effect of pressure, in the equation two there is no effect of pressure. So, by simple seeing the reaction, it is clear that if I decrease the partial pressure of carbon monoxide, then the carbon oxidation will be favored. So, what is the solution, now, to those two challenges. The solution is reduction in partial pressure of carbon monoxide. Now, how this reduction of partial pressure of carbon monoxide can be done? Say, it is easy, but then, it is to be done, it is to be practiced, it is to be used and then you have to produce stainless steel at the economic cost. That is the important because, that technology which is economical, which will work. Otherwise, that will lose its significance. How to reduce partial pressure of carbon monoxide? One way, we use vacuum. That is vacuum oxygen decarburization process. Very expensive to employ vacuum and then to carry out the stainless steel making; however, for various special quality this process is being adopted. Another is that, we use argon plus oxygen mixture. Imagine, if I take now, a mixture of argon and oxygen, instead of pure oxygen, then argon will react as a diluents and it will decrease the partial pressure of carbon monoxide. So, this particular process, using argon and oxygen mixture has become very popular and this process is known as A O D, A stands for argon O stands for oxidation and D stand for decarburization. So, the whole process is known argon oxygen decarburization process. Now, let us see what this process is.
10 (Refer Slide Time: 22:53) So, argon oxygen decarburization process. Now, in this process, the iron, chromium, carbon, nickel melt is prepared as usual in electric arc furnace; that means, this argon oxygen decarburization process works in combination with electric arc furnace. So, the input of this argon oxygen decarburization process is the output of electric arc furnace and the output of electric arc furnace is a melt which contains iron, chromium, carbon, nickel melt is prepared in the electric arc furnace. Tapping temperature is 1500 to 1600 degree Celsius, charged in A O D vessel. Here high carbon ferrochrome is used to prepare stainless steel. So, typically I have shown A O D converter. So, it is again a pear shaped vessel, lined with basic magnesite lining. Now, the important point in this A O D vessel is that, these vessels are side blown. On the side of the converter, there are 4 to 6 or 8 tiers are arranged and a mixture of oxygen plus argon is blown into the vessel. Those heats which can tolerate nitrogen, then a mixture of oxygen and nitrogen can also be blown. But to start with, if those heats which cannot tolerate the nitrogen content in steel, then you have to blow argon, in order to reduce the partial pressure of carbon monoxide. So, how this is done? Iron, chromium, carbon, nickel melt from electric furnace is transferred to the A O D vessel. High carbon ferrochrome is added and the blow begins with the blowing of argon and oxygen mixture.
11 (Refer Slide Time: 26:08) Now, typically, in the beginning, oxygen is to argon ratio is kept 3 is to 1; that is, in the beginning until carbon reduces to around 30 percent. Now, since they are blowing along with the argon, so, it is possible to carry out decarburization at a lower temperature also. Now, when carbon is reduced to 30 percent, then oxygen to argon ratio is decreased to 2 is to 1. Now, decrease the oxygen, because you require less oxygen for the oxidation of carbon and the bath is blown to 0.09 to 0.12 percent carbon. So, if you call this as a stage 1, this is stage 2. Then in stage 3, the oxygen to argon ratio is 1 is to 2, to bring carbon content of bath to the desired value, could be or whatever. So, this is the blowing schedule of a typical argon oxygen decarburization converter in order to produce a stainless steel. The main point to understand over here is, a mixture of argon and oxygen is blown and that mixture does the job of removal of carbon at lower temperature. Now, major change in this practices is occurred in the last few years. That is instead of argon, those heats which can tolerate little amount of nitrogen, nitrogen can also be blown. However, some degassing is also possible in the stage 3, some amount of nitrogen can also be removed. Some manifestation, say, first stage blow it generates heat and a coolants of the order of 5 to 10 percent of the coolant, they are added. Stainless steel as a coolant is better. The cooling or the coolant addition is done during first stage, when temperature rises to 1690 or 1700 degree Celsius. When carbon has been removed, then ferrosilicon is added to
12 recover lost chromium into slag, back to the metal. Because, when a mixture of oxygen argon is blown, some amount of chromium will also be oxidized in the beginning and that chromium as C r 2 O 3 it collects in the slag. Now, the most important is decarburization. Let little amount of chromium, if it oxidizes, let it oxidize, because then it can be recovered by addition of ferrosilicon and that is being done in the practice. When carbon is come down to the specification, then ferrosilicon is added to recover chromium oxide. Basicity of slag is maintained at around 1.5 to 2 and the reaction is C r 3 O 4 plus 2 silicon that gives 3 C r plus 2 S i O 2. (Refer Slide Time: 30:50) The chromium recovery it may vary, but some figure like 97 percent chromium can be recovered from the slag, back to the metal. Some sort of desulphurization can also be achieved, if the need arises. If very low nitrogen content in stainless steel required, then nitrogen blowing is not done. If little amount of nitrogen can be tolerated by stainless steel, then nitrogen blowing is being done. So, this is about the production of stainless steel by A O D and electric arc furnace. Now, this particular lecture concludes on modern steel making processes. Now, as a concluding remark, I have to say the following. In the coming years the production of steel by electric arc furnace will grow. For very simple reason, if you compare with the root, coke oven, blast furnace and B O F, which is valid for integrated steel plant, the production of steel by electric arc furnace can be, can be done at a very competitive
13 price. So, in the years to come the production of steel by electric arc furnace is going to grow; that means, the developments in electric arc furnace will continue to grow in the following direction. The first development that you will see, use of ultra-high power input. For example, up to 1500 kilo volt ampere per ton of power input is envisaged. Second development is, improved furnace and equipment design features. Third, refining combined burner technology, burner technology for enhanced E A F performance, through oxygen injection, carbon injection or through natural gas burner injection; these are bound to come. So, for example, a 120 ton ultimate electric arc furnace is capable of increase in 50 percent capacity, roughly equivalent to 180 tons, by incorporating these above mentioned modern gadgets. Also, the developments will go on in using the furnace for different charge mixes, starting from 100 percent scrap to a combination of a scrap D R I, H B I and hot metal. (Refer Slide Time: 34:52) Now, I will give you some key data of ultimate E A F installations. For example, I put here, the some company, Reveda, Betrosorsky in Russia, that is one company, then Atoun Steel in Saudi-Arabia and Reveda company in Russia, they have installed three most modern electric arc furnaces. Their specifications are as follows: one, tapping weight in tons, it is 120, here it is 80, here it is 165. Furnace diameter 7.7 meter, 6.5 meter and 8.6 meter. Transformer, please note the transformer capacity. Transformer, here it is 150 mega volt ampere; then this correspond to 1250 kilo volt ampere per ton.
14 This furnace is operating. Here it is 105 mega volt ampere, which correspond to 1313 kilo volt ampere per ton and here it is 195 mega volt ampere, which correspond to 1182 kilovolt ampere per ton. So, you can see now, some plants are already working with the modern gadgets, having ultra-high power furnaces. Now, these ultra-furnaces, they have injection tools. This company have 5 R C B, that is refining combined burner plus 2 burners, 4 post combustion system, plus 4 carbon injectors. Appears to be the most modern furnace. This one is having 3 R C B plus 2 burners, 2 post combustion system, 2 carbon injectors, may be because its capacity is low. Third one has 5 R C B, 3 burners, you know the burners are used for meltdown period, natural gas and oxygen mixture, 4 post combustion systems and 4 carbon injectors. Now, what is the ultimate objective of employing these modern gadgets? The ultimate objective is to have a tap to tap time parallel to B O F steelmaking. You remember, a B O F steelmaking or a B O F converter taps 300 to 400 tons of steel in just a matter of 60 minutes. Compared to electric arc furnace, which used one and half to 2 hours. So, the whole idea of employing these gadgets, is to make the electric arc furnace competitive with reference to tap to tap time and these modern gadgets made possible, if I write now tap to tap time, in all the cases is 36 minutes. (Refer Slide Time: 39:46)
15 So, you can imagine, where the electric arc furnace development will lead to. Ultimately, it will be parallel to B O F steelmaking. So, here are some questions, that is selfassessment questions in B O F steelmaking. Question one, what is the principle of steelmaking? Write the chemical reactions as already I have said, you have to write down. Second, what are the essential requirements of a L D steel melting shop? Briefly explain the logistics. (Refer Slide Time: 40:16) I explained to you already. Third, describe the design features of a converter. Explain the importance of working height in the converter. You know already. Fourth, how oxygen is supplied to refine hot metal in L D converter? This has also been explained in the form of the jet, free-jet and momentum flow rate and so on. Question number fifth, what are the functions of nozzle in the method of oxygen supply described in question 4? Nozzle, it converts a given flow rate of the jet into energetic supply and I have already described 4 or 5 functions, that you have to bring it over to here. 6, what is a gaseous jet? Briefly describe the behavior of jet, when it is discharged in a surrounding of a cold air, hot air and slag metal emulsion. Here, you have to bring the ratio of density of jet to density of surrounding. 7, what are the feed materials? That already I have said. Eighth, what is the mechanism of refining of hot metal in L D converter? You recall, I have superimposed lance profile with the physico-chemical interaction between the jet and bath, you can bring it over here.
16 (Refer Slide Time: 41:03) Question 9, explain the cause of increase in manganese. 10, what is catch carbon practice? 11, discuss the mechanism of foams and emulsion formation in L D steelmaking. This is, also, I have already described. Twelfth, what factors affect lining life and 13, 14 and 15, they rather addresses or these questions have been formulated to know what are the different technologies available for repairing of the lining. (Refer Slide Time: 41:31) The questions of electric arc furnace steelmaking. What is a foaming slag? Explain the formation of foamy slag. Discussed. What is the role of oxygen lancing? Also discussed.
17 What is an oxy-fuel burner? Oxy-fuel burner is used in the melt down period to increase the rate of melting and to attain quick (( )) bath condition. Explain how the metallurgical quality of D R I and H B I affects the electric power consumption in E A F. I have discussed, I have calculated some values also. An E A F is operating with 100 percent scrap. What modification would be required to use chemical energy? A modification would be, either you inject carbon or you inject oxygen, because for utilizing chemical energy, you have to have chemical reaction. What is the equivalent carbon in D R and what is its significance? Already I have calculated the carbon content in D R I and stoichiometric, all this thing you have to bring over to here. (Refer Slide Time: 42:26) Question 7, what are the requirements of injection of oxygen for decarburization and post combustion in E A F steelmaking? Discussed. Calculate the amount of C O and oxygen required generating chemical energy 30 kilo watt hour per ton of steel. You have to write down the reaction C O plus half O 2 is equal to C O 2, find out the heat of formation and make it equivalent to 30 kilo watt hour per ton, so that, you can calculate how much amount of C O will be required. Discus the mechanism of foaming. Explain the physico-chemical principles of stainless steel manufacture. This I have discussed right now. Discuss the importance of carbon boil. How do you promote the carbon boil by injecting carbon also thing I have been discussed. Name the sources of C O and hydrogen generation in E A F steelmaking.
18 (Refer Slide Time: 43:10) (Refer Slide Time: 43:18) Now, these are the references which you can consult. The lecture has been prepared from these references, plus these references
Steel Making Prof. Deepak Mazumdar Prof. S. C. Koria Department of Materials Science and Engineering Indian Institute of Technology, Kanpur Module No. # 01 Lecture No. # 16 Modern Steelmaking II, Electric
Steel Quality Role of Secondary Refining and Continuous Casting Dr. Santanu Kr Ray Department of Mechanical Engineering Indian Institute of Technology, Madras Module - 02 Lecture - 06 Limitation of Primary
Lecture 12 Converter Steelmaking Practice & combined blowing Contents: Refining of hot metal Composition and temperature during the blow Physico-chemical interactions Developments in Top blown steelmaking
Use of DRI in EAF s Gregory L. Dressel Dressel Technologies Pawleys Island, SC Part III: Slag Practices and Oxygen/Carbon Injection when Melting Direct Reduced Iron Introduction When melting DRI or HBI
PYREJET A MULTI-FUNCTION COMBUSTION/INJECTION SYSTEM FOR EAF STEELMAKING ACI has developed a PyrJet a new proprietary multi-functional burner/injection system for the Electric Arc Furnace (EAF). The new
Steel Making Prof. Deepak Muzumdar Prof. S.C. Koria Department of Material Science and Engineering Indian Institute of Technology, Kanpur Module No. # 01 Lecture No. # 25 Deoxidation, Ladle and Tundish
EAF Technology and process In the last 100 years,the EAF technology has evolved to meet the demands of higher productivity, improved quality of product and flexibility of metallic inputs. The product mix
Steel Making Prof. Deepak Muzumdar Prof. S. C. Koria Department of Material Science and Engineering Indian Institute of Technology, Kanpur Module No. # 01 Lecture No. # 01 Introduction So, I welcome you
Steel Making Prof. Deepak Mazumdar Prof. S. C. Koria Department of Materials Science and Engineering Indian Institute of Technology, Kanpur Module No. # 01 Lecture No. # 04 The Science Base of Iron and
EFFICIENT VACUUM CONVERTER FOR INDIVIDUAL NEEDS Refined steels and ferroalloys SMS group X-Melt Vacuum Converter X-MELT VACUUM CONVERTER Producing special steels and ferroalloys SMS group has specially
Lecture 14 Modern trends in BOF steelmaking Contents: Post combustion Technology of post combustion Potential post combustion issues Slag splashing What is required for slag splashing Liquidus temperature
Lecture 21: Evolution of ladle Treatment and Requirements Contents: Preamble What modifications are required? Basics of gas stirring Mixing time Gas injection rates Choice of stirring energy Key words:
Chapter 2 Electric Arc Furnace as Thermoenergetical Unit 2.1 Thermal Performance of Furnace: Terminology and Designations There are different forms of energy. Heat is one of them. Heat is a form of energy
Extracting Metals Which country is the leading producer? Copper Philippines Chile Gold China Nickel Mexico Platinum Titanium Silver South Africa Australia Diamond Australia, Chile, China, Mexico, Philippines,
IRONMAKING and STEELMAKING THEORY AND PRACTICE Ahindra Ghosh Amit Chatterjee IRONMAKING AND STEELMAKING IRONMAKING AND STEELMAKING Theory and Practice AHINDRA GHOSH Formerly Professor Materials and Metallurgical
Yuri N. Toulouevski Ilyaz Y. Zinurov Innovation in Electric Arc Furnaces Scientific Basis for Selection The Second Edition Revised and Supplemented ^ Springer Contents 1 Modem Steelmaking in Electric Arc
NOVEMBER 2012 POLYMER INJECTION TECHNOLOGY ONESTEEL NSW Pty Ltd appoints world-leading supplier MORE to promote Polymer Injection. OPERATIONAL RESULTS AT NUNKI STEEL Nunki Steel S.p.A. is located in San
Lecture 42: Self Assessment questions 1a) Explain the role of a basic oxidising slag in steelmaking. (04) 1b) Carry-over of the basic oxidising slag from the converter is undesirable to the transfer ladle.
Iron and Steel Manufacturing 40 CFR Part 420 Description of the Industry Three basic types for facilities Integrated steel mills Non-integrated steel mills Stand-alone facilities Iron and Steelmaking Operations
10 Sulphur Problem AkMB Rashid Professor, Department of MME BUET, Dhaka Today s Topics Introduction Behaviour of sulphur in metal and slag Oxidation of sulphur in the furnace Oxidation of sulphur in the
Optimization of EAF Operations Through Offgas System Analysis Jeremy Jones 1 Paykan Safe 2 Brian Wiggins 2 1 Nupro Corporation, Grand Island N.Y. 716-773-8726 716-773-8735 Fax 2 Gas Cleaning Technologies,
1 Iron from a blast furnace is treated with and with calcium oxide to make steel. Which substances in the are removed? removes calcium oxide removes acidic oxides basic oxides acidic oxides basic oxides
Lecture 25: Principles of degassing Contents Introduction Principles Side reactions General considerations Fluid flow in degassing Material balance in de gassing Key words: Degassing, gases in steel, ladle
MODULE DESCRIPTOR TITLE MATERIALS PROCESSIG SI MODULE CODE 16-6279 CREDITS 20 LEVEL 6 JACS CODE J510 SUBJECT GROUP Materials Engineering DEPARTMET Engineering and Mathematics MODULE LEADER Dr Antonio Feteira
Improvement of energy efficiency in EAF steelmaking With ever increasing costs for electricity and the environmental penalty from the production of CO 2 during steelmaking, plant operators must continuously
Choosing the Right Technologies for Reverb Furnaces Russell Hewertson, Manager of Combustion Technology Choosing the Right Technologies for Reverb Furnaces Russell Hewertson, Manager of Combustion Technology
Welding Engineering Prof. Dr. D. K. Dwivedi Department of Mechanical and Industrial Engineering Indian Institute of Technology, Roorkee Module - 4 Arc Welding Processes Lecture - 1 SMAW- 1 So, dear students,
Use of DRI in EAF s Gregory L. Dressel Dressel Technologies Pawleys Island, SC Part II: Feeding and Melting of Direct Reduced Iron Introduction Perhaps the most important consideration an operator gives
, pp. 413 418 Conversion of CO 2 Gas to CO Gas by the Utilization of Decarburization Reaction during Steelmaking Process Hiroyuki MATSUURA* and Fumitaka TSUKIHASHI Department of Advanced Materials Science,
Title How to make the plants of today comply with the requirements of tomorrow Authors Dr. Christian Fröhling General Manager Energy and Environmental Technology Dr. Peter Hemmling Senior Specialist Energy
IRON AND STEEL INDUSTRY DEVELOPMENT AND TECHNOLOGICAL INNOVATION IN CHINA Kuang-di Xu Chinese Academy of Engineering, China ABSTRACT China s iron and steel industry enjoys accelerated development thanks
U.P.B. Sci. Bull., Series B, Vol. 75, Iss. 2, 2013 ISSN 1454-2331 REFINING STEELS PRODUCED IN ELECTRIC ARC FURNACE Valentin MINCU 1, Nicolae CONSTANTIN 2 Characteristics and properties of cast and forged
MELTING PROCESS INTENSIFICATION AT 20 t EAF - ŽĎAS, A.S. Pavel Fila, Oldřich Suchý, Martin Balcar, Ludvík Martínek a, Jaroslav Brhel, Aleš Kosek b a) ŽĎAS, a.s. Strojírenská 6, 59171 Žďár nad Sázavou b)
1 Pyrometallurgy of iron is still the most important pyrometallurgical process economically. Prehistorically, iron was prepared by simply heating it with charcoal in a fired clay pot. Coke is coal that
1 DEPHOSPHORIZATION AND DESULFURIZATION OF MOLTEN DUCTILE IRON AND ITS EFFECT ON DUCTILITY By Rub Nawaz Ansari (Deputy Manager, Bolan Castings Ltd. Pakistan) PROBLEM: The importance of phosphorus in the
Development of Recycling and Melting Technology Using the -based FASTMELT Process By M. Tateishi, H. Fujimoto, T. Harada, H. Sugitatsu Kobe Steel, Ltd. Editor s note: this article was adapted from a paper
1 P age Module 4: Gaseous Fuel Lecture 28: Water Gas 2 P age Keywords: Coal gasification, steam blast, blast saturation temperature, gas generator 4.3 Water gas Water gas is a gaseous fuel generated in
Metallurgy and lining life in basic oxygen converters Good control of slag development, oxygen flow and lance practice, and use of bottom stirring and re-blow practice are key aspects of the metallurgical
STAINLESS STEEL MANUFACTURING PROCESS 1. INTRODUCTION 2. MELTING SHOP 3. HOT ROLLING SHOP 4. COLD ROLLING SHOP 1. INTRODUCTION CONVERT RAW MATERIALS IN FINAL PRODUCTS (COILS AND SHEETS) RAW MATERIALS YARDS
ET3034TUx - 4.2 - Manufacturing of crystalline silicon We have various types of silicon wafers such as monocrystalline silicon and polycrystalline silicon. In this block I will give an answer to the question:
Multilayer Perceptron to Model the Decarburization Process in Stainless Steel Production Carlos Spínola 1, Carlos J Gálvez-Fernández 1, José Muñoz-Pérez 2, José Mª Bonelo 3, Javier Jerrer 4, Julio Vizoso
ABSTRACT MASS AND HEAT BALANCE OF STEELMAKING IN BOF AS COMPARED TO EAF PROCESSES M.M.LOTFY 1, H.A.AHMED 2 AND F.A.ELREFAIE 3 Mass and energy balance equations are applied on top blowing BOF and EAF steelmaking
THE MOST ADVANCED POWER SAVING TECHNOLOGY IN EAF INTRODUCTION TO ECOARC T. Nagai, Y. Sato, H. Kato, M. Fujimoto and T. Sugasawa JP Steel Plantech Co., Yokohama, Japan Contact data T. Nagai, JP Steel Plantech
CPC - C21C - 2017.05 C21C PROCESSING OF PIG-IRON, e.g. REFINING, MANUFACTURE OF WROUGHT- IRON OR STEEL; TREATMENT IN MOLTEN STATE OF FERROUS ALLOYS (refining metals in general C22B 9/00) all treatments
Rolling Process Metallurgical Aspects Material Specifications and Chemistries Standard Mill Practices Miscellaneous Tables & Data Elastic Section Modulus Plastic Section Modulus Moment of Inertia SI Conversion
Missouri University of Science and Technology Scholars' Mine Materials Science and Engineering Faculty Research & Creative Works Materials Science and Engineering 1-1-2005 Alloy Recovery and Control in
Revision from Year 10: Properties of Metals and Non-Metals Read CC pp182-183 Use arrows to link the properties with the materials: Strong under tension and compression Malleable Low density Have a dull
Non-ferrous Extractive Metallurgy Prof. H. S. Ray Department of Metallurgical and Materials Engineering Indian Institute of Technology, Kharagpur Module No. # 01 Lecture No. # 10 Refining of Metals - Chemical
INTRODUCTION PROCESS TECHNOLOGY CONFERENCE PROCEEDINGS VOLUME 11 ATLANTA, GA 1992 Ultra-Refining Processes for Specialty Steelmaking A PUBLICATION OFTHE IRON AND STEEL SOCIETY Reprinted from 11th Process
2.7 EXTRA QUESTIONS MS 1. (a) C + Cl 2 (or in eq n ) (1) heat or 500 1000 C (1) 2 (b) electrolysis (1) molten or with cryolite (1) 2  2. Equation(s) for iron Fe 2 O 3 + 3C 2Fe + 3CO (1) (3CO) (3CO 2
Operating results of Goodfellow EFSOP at Riva Galtarossa, Italy The installation of two Goodfellow EFSOP systems at Riva Acciaio SpA has resulted in improved electric arc furnace performance in terms of
Briquette Smelting in Electric Arc Furnace to Recycle Wastes from Stainless Steel Production Qi-xing YANG 1 2 2, Dong-feng HE 2 3 1 Abstract: Wastes from stainless steel production were briquetted together
Twinjection Technology Improves Hot Metal Desulphurisation at Corus Scunthorpe Works Dr. Robert Robey, Process Metallurgist, Mark Whitehead, Manager - Technical Sales, SMS Mevac UK Limited, Winsford, UK;
A. Stainless Steel o Electric Are Furnace (EÃF) Accurate end-point control begins in the EAF. Chapter IV AOD Processing That statement is not surprising, but it deserves emphasis. It is very easy to relax
MASTER'S THESIS Thermodynamic Study of Trace Elements in the Blast Furnace and Basic Oxygen Furnace Anton Andersson 2014 Master of Science in Engineering Technology Sustainable Process Engineering Luleå
MODULETECHNOLOGY 26 27 MODULE TECHNOLOGY OXYGEN, CARBON AND LIME SIDE WALL INJECTION TECHNOLOGY FOR ELECTRIC ARC FURNACES CONCEPT The MODULE TECHNOLOGY: state-of-the-art chemical energy package for electric
Manufacturing Process - I Prof. Dr. D.K. Dwivedi Department of Mechanical & Industrial Engineering Indian Institute of Technology, Roorkee Module - 3 Lecture - 11 Tungsten Inert Gas Welding Part 1 Welcome
Q1. Iron is extracted from iron oxide in the blast furnace. (a) The equation for one of the reactions in the blast furnace is: Fe 2 O 3 + 3CO 2Fe + 3CO 2 Complete the word equation for this reaction. iron
76 BENEFIT OF GAS PURGING IN BOF AND EAF WITH A FOCUS ON MATERIAL EFFICIENCY AND EMISSION REDUCTION. Thomas Kollmann, Marcus Kirschen, Christoph Jandl, Karl-Michael Zettl RHI AG, Vienna Abstract In highly
Smart-Gas A New Approach to Optimizing EAF Operations Jeremy A.T. Jones Nupro Corporation, 755 Center Street, Suite 3, Lewiston, New York, 14092, 716-754-7770, firstname.lastname@example.org Sam Matson WorleyParsons
Session II: DRI in focus DRI in use: How can DRI (HBI) be utilized in the Blast Furnace and BOF? by Ralph Smailer, Director/Owner Metserv Ironmaking and Steelmaking Practices with HBI Blast Furnace Practice
, pp. 24 28 Analysis of Droplet Generation in Oxygen Steelmaking Neslihan DOGAN, Geoffrey BROOKS and Muhammad Akbar RHAMDHANI Faculty of Engineering and Industrial Science, Swinburne University of Technology,
MGO-C REFRACTORY SELECTION AND EVALUATION FOR STEELMAKING VESSELS Arcelormittal Abstract The challenge for refractory material producers and consumers is to find the optimum solution between the quality
OPERATING EXPERIENCE AT A 170 t EAF WITH EPC SCRAP PREHEATING SYSTEM BY KNUT RUMMLER* DR. HEINZ MÜLLER** INTRODUCTION In the recent years, the growth of EAF steelmaking and the corresponding push for improved
Final Technical Report Project Title: Melting Efficiency Improvement Award Number: DE-FC36-04GO14230 Project Period: (January 2004 June 2012) Principal Investigator: Kent Peaslee, 573-341-4714, email@example.com
GSMPM BLOW CHARGE MODEL IMPLEMENTATION AT ARCELORMITTAL TUBARÃO* Henrique Silva Furtado 1 Lourival Silva Machado 2 Roberto Dalmaso 3 Abstract This paper presents the results obtained on the exchange of
Importance and Effect of Foaming Slag on Energy Efficiency T.M. Kipepe, X. Pan Department of Extraction Metallurgy, Faculty of Engineering and the Built Environment, University of Johannesburg Johannesburg,
self evaluation self evaluation 1.Stannite deposits constitute an important source for which of the following metal a) Thorium b) Titanium c) Molybdenum d) Tin 2. In mineral beneficiation a) Mineral is
International Journal of Scientific & Engineering Research Volume 2, Issue 10, October-2011 1 How to make N 2 listen to you in steel making! P R Sureshkumar, D R Pawar and V Krishnamoorthy Abstract- All
Project partners Workshop Road map for future EAF technology Sensors and measurement techniques for monitoring and control of the EAF process Dr. H. Köchner, VDEh-Betriebsforschungsinstitut (BFI), Düsseldorf,
EAF REFRACTORY PERFORMANCE AT PACIFIC STEEL NEW ZEALAND Don Sanford Product Manager Refractories Chemiplas, New Zealand Ltd Level 2, 42 Upper Queen Street Auckland, New Zealand DonS@chemiplas.co.nz Brian
4th International Conference on Molten Slags and Fluxes, 1992, Sendai, ISIJ A DYNAMIC SLAG-DROPLET MODEL FOR THE STEELMAKING PROCESS v v 'f. W. van der Knoop~ Brahma Deo, A.B. Snoeijer~ G. van Unen"" and